Presentation on theme: "Lec. (4, 5) 1. These approaches use larger (macroscopic) initial structures, which can be externally-controlled in the processing of nanostructures. Typical."— Presentation transcript:
Lec. (4, 5) 1
These approaches use larger (macroscopic) initial structures, which can be externally-controlled in the processing of nanostructures. Typical examples are etching through the mask, ball milling, and application of severe plastic deformation. These approaches include the miniaturization of materials components (up to atomic level) with further selfassembly process leading to the formation of nanostructures. During self-assembly the physical forces operating at nanoscale are used to combine basic units into larger stable structures. Typical examples are quantum dot formation during epitaxial growth and formation of nanoparticles from colloidal dispersion. Bottom-up approach Top-down approach There are two general approaches to the synthesis of nanomaterials and the fabrication of nanostructure 2
Top-Down: lithography At the moment, the most used top-down approach is photolithography. It has been used for a while to manufacture computer chips and produce structures smaller than 100 nm. Typically, an oxidized silicon (Si) wafer is coated with a 1μm thick photo-resist layer. After exposure to ultraviolet (UV) light, the photoresist undergoes a photochemical reaction, which breaks down the polymer by rupturing the polymer chains. Subsequently, when the wafer is rinsed in a developing solution, the exposed areas are removed. A beam of UV light activates the photoresist, transferring the pattern from the mask to the sample. 4
Photolithography 5 Coat, protect, expose, etch, repeat… result in Multiple patterned layers of different 5 materials.
6 Is the most recent lithography methods. Printing, stamping, and molding use mechanical processes instead of photons or electrons. These methods are normally called soft lithography methods because they involve the use of polymers.
7 Though the concept of photolithography is simple, the actual implementation is very complex and expensive. This is because (1) nanostructures significantly smaller than 100 nm are difficult to produce due to diffraction effects. (2)masks need to be perfectly aligned with the pattern on the wafer. (3) the density of defects needs to be carefully controlled, and (4) photolithographic tools are very costly, ranging in price from tens to hundreds of millions of dollars. Once the master template has been made, no special equipment is required. Soft lithographic methods are capable of producing nanostructures in a wide range of materials and can print or mold on curved as well as planar surfaces
9 Principal: Gas –phase precursors interact with a liquid–or solid-phase material Gas state condensation Chemical vapor deposition Molecular beam epitaxy Atomic layer deposition Combustion Thermolysis Metal oxide vapor phase epitaxy Ion implantation
10 The inert gas condensation (IGC) process is one of the most known and simplest technique for production of nano-particles.
11 1. A material, often a metal, is evaporated from a heated metallic source into a chamber which has been previously evacuated to about 10–7torrand backfilled with inert gas to a low-pressure. 2. The metal vapor cools through collisions with the inert gas atoms, becomes supersaturated and then nucleates homogeneously; the particle size is usually in the range 1–100 nm and can be controlled by varying the inert gas pressure. 3. Ultimately, the particles are collected and may be compacted to produce a dense nanomaterial.
Physical Vapor Deposition (PVD)
a)Thermal evaporation (resistively, electron beam) b)Sputtering (gas ion bombardment) c)Pulsed laser deposition (laser beam)
Chemical Vapor Deposition (CVD) Laser beam or plasma can be introduced to enhanced the reaction Can fabricate: carbon nanotubes, inorganic oxide nanorods, nanowire etc. Source material /carrier gas Principal: CVD involves the formation of nanomaterials from the gas phase at elevated temperatures—usually onto a solid substrate or catalyst. Heater
4. Purge or evacuation of the reaction chamber. Each reaction cycle adds a given amount of material to the surface, referred to as the growth per cycle. reaction cycles are repeated to reache the desired film thickness. The growth of material layers by ALD consists of repeating the following characteristic four steps: 1.Exposure of the first precursor, typically an organometallic compound.organometallic 2.Purge or evacuation of the reaction chamber to remove the non-reacted precursors and the gaseous reaction by-products. 3. Exposure of the second precursor – or another treatment to activate the surface again for the reaction of the first precursor, such as a plasma.plasma Atomic layer deposition
Vacuum arc deposition is well-established process for producing of thin films and nanoparticles. This technique involves the initiation of an arc by contacting a cathode made of a target material. An igniter is attached to an anode in order to generate a low-voltage, high-current self-sustaining arc. The arc ejects ions and material droplets from a small area on the cathode. Further, the ions are accelerated towards a substrate while any large droplets are filtered out before deposition. Plasma Based Synthesis
Vapour Condensation One of the outstanding strides in plasma processing for nanoparticles synthesis is the developed process of the vapor condensation. The precursor material is put into the working chamber with a stable arc. The chamber is filled by reactive gas that becomes ionized; then molecular clusters are formed and cooled to produce nanoparticles.
The production route for 1-D rod-like nanomaterials by liquidphase methods is similar to that for the production of nanoparticles. CVD methods have been adapted to make 1-D nanotubes and nanowires. Catalyst nanoparticles are used to promote nucleation. Nanowires of other materials such as silicon (Si) or germanium (Ge) are grown by vapor-liquid-solid (VLS) methods. Methods for making 1-D and 2-D nanomaterials
20 Molecular Beam Epitaxy (MBE) A molecular beam epitaxy (MBE) machine is essentially an ultra-high-precision, ultra clean evaporator, combined with a set of in-situ tools, such as Auger electron spectroscopy (AES) and/or reflection high- energy electron diffraction (RHEED), for characterization of the deposited layers during growth.
21 Schematic diagram of a molecular beam epitaxy thin film deposition Molecular Beam Epitaxy (MBE)
22 In solid-source MBE, ultra-pure elements such as gallium and arsenic are heated in separate quasi-Knudsen effusion cells until they begin to slowly evaporate. The evaporated elements then condense on the wafer, where they may react with each other. In the example of gallium and arsenic, single crystal gallium arsenide crystal is formed. The term “beam” simply means that evaporated atoms do not interact with each other or any other vacuum chamber gases until they reach the wafer, due to the long mean free paths of the beams. The substrate is rotated to ensure even growth over its surface. By operating mechanical shutters in front of the cells, it is possible to control which semiconductor or metal is deposited. The sources can be either solid or gaseous and an MBE machine will typically have an array of multiple sources, which can be shuttered to allow layered, alternating heterostructures to be produced. Semiconductor quantum wells, superlattices and quantum wires and metallic or magnetic multilayers for spin valve structures are deposited using this technique.
23 Atomic Layer deposition (ALD)
24 Bottom up method of Atomic Layer deposition (ALD) 1. High precision actuators move atoms from place to place 2. Micro tips emboss or imprint materials 3. Electron (or ion) beams are directly moved over a surface 1. Chemical reactors create conditions for special growth 2. Biological agents sometimes used to help process 3. Materials are harvested for integration
Template-based Methods Just name a few Biosensor Chemical sensor Drug delivery Self-cleaning Energy harvesting … Applications
The sol is a name of a colloidalsolutionmade of solid particles few hundred nm in diameter, suspended in a liquid phase. The gel can be considered as a solid macromolecule immersed in a solvent. + Sol-gel process consists in the chemical transformation of a liquid (the sol) into a gel state and with subsequent post-treatment and transition into solid oxide material. The main benefits of sol–gel processing are the high purity and uniform nanostructure achievable at low temperatures.
Electrodeposition is a long- established way to deposit metal layers on a conducting substrate. Ions in solution are deposited onto the negatively charged cathode, carrying charge at a rate that is measured as a current in the external circuit. The process is relatively cheap and fast and allows complex shapes. The layer thickness simply depends on the current density and the time for which the current flows. The deposit can be detached if the substrate is chosen to be soluble by dissolving it away.
The principle of electrodeposition is inducing chemical reactions in an aqueous electrolyte solution with the help of applied voltage, e.g. this is the process of using electrical current to coat an electrically conductive object with a relatively thin layer of metal. Electrodeposition Electrodeposition is relatively cheap and can be performed at low temperatures which will minimize interdiffusion of materials in the case of a multilayered thin film preparation. The film thickness can be controlled by monitoring the amount of charge delivered, whereas the deposition rate can be followed by the variation of the current with time. The composition and defect chemistry can be controlled by the magnitude of the applied potential, which can be used to deposit non-equilibrium phases. Electrodeposition advantages
The insulating mask need not have a straight line-of-sight path between the substrate and the electrolyte; even tortuous masks can be filled with materials, so long as the whole path through the mask is wetted with the ED electrolyte. The resulting deposit is a high fidelity negative replica of the mask itself. Through-mask ED has been used extensively to pattern metals, semiconductors, and polymers on conductive substrates. Electrodeposition in microelectronics A ten level copper on-chip interconnect scheme of 90 nm CMOS node fabricated in low dielectric constant material.